Biodeterioration of Construction Materials: State of the Art and Future Challenges
M. Sanchez-Silva, A.M.ASCE1; and David V. Rosowsky, P.E., M.ASCE2
Abstract: Deterioration plays an important part in the life cycle of infrastructure systems. Among all causes of deterioration aging, chloride ingress, etc. the action of live organisms has shown to be critical in, for example, underground structures, sewage systems, and at-sea structures. This phenomenon is usually overlooked, in part, because in most cases live organisms accelerate other processes that may eventually lead to unacceptable structural performance or cause failure e.g., corrosion, cracking. By the direct or indirect action, it has been estimated that biodeterioration-related structural problems cost billions of dollars a year in infrastructure maintenance and repair. The paper shows that for all major civil engineering materials, in the long term and under the appropriate environmental conditions, biodeterioration may severely affect infrastructure components and their ability to perform as designed. This is particularly relevant given the large amount of existing infrastructure that has been exposed to aggressive environments for long periods of time. This paper presents an overview of the activity of live organisms on three widely used construction materials: wood, concrete, and metals. A description of the main organisms that affect each material and the associated biodeterioration mechanisms are described. In addition, this paper discusses the uncertainties associated with modeling biodeterioration and outlines the main areas for further research.
CE Database subject headings: Deterioration; Concrete; Wood; Metals; Uncertainty principle; Construction materials.
A comprehensive life-cycle cost analysis should take into consid- eration all factors that might cause a structural system to perform unacceptably at any point during its lifetime. This includes ex- treme events e.g., earthquakes, cyclones or the progressive and sustained loss of capacity caused by operation or environmental factors. The latter has perhaps the broadest impact on the long- term performance of infrastructure systems and the largest poten- tial economic consequences. Within this context, it has been observed that biodeterioration of structural materials may contrib- ute significantly to continued loss of capacity of some structures located in aggressive environments. For instance, it is well known that it plays a significant role in the deterioration of structures in which wood is the major component. However, relatively little attention has been given to biodeterioration in large infrastructure systems where reinforced concrete and steel are the dominant constitutive materials.
1Visiting Scholar, Zachry Dept. of Civil Engineering, Texas A&M Univ., College Station, TX 77843-3136. E-mail: [email protected]
civil.tamu.edu; Associate Professor, Dept. of Civil and Environmental Engineering, Univ. de Los Andes, Carrera 1, No. 19A-40 Edificio Mario Laserna, Piso 6, Bogotá, Colombia. E-mail: [email protected]
2Department Head and A.P. and Florence Wiley Chair Professor, Zachry Dept. of Civil Engineering, Texas A&M Univ., 3136 TAMU, College Station, TX 77843-3136 corresponding author. E-mail: [email protected]
Note. Associate Editor: Hilary I. Inyang. Discussion open until October 1, 2008. Separate discussions must be submitted for individual papers. To extend the closing date by one month, a written request must be filed with the ASCE Managing Editor. The manuscript for this paper was submitted for review and possible publication on September 7, 2006; approved on July 18, 2007. This paper is part of the Journal of Materials in Civil Engineering, Vol. 20, No. 5, May 1, 2008. ©ASCE, ISSN
352 / JOURNAL OF MATERIALS IN CIVIL ENGINEERING © ASCE / MAY 20
Biodeterioration occurs at the boundary between engineering and biology usually microbiology. Therefore, it is necessary to consider both the physical and chemical mechanisms by which microorganisms attack the material, and the consequences on its mechanical properties. In wood, the mechanical properties of the material are altered mainly by live organisms that use it as a food source. In concrete structures biodeterioration affects the concrete matrix increasing porosity and contributing to crack growth. In metals placed in aggressive environments i.e., at sea, microor- ganisms contribute significantly to the corrosion process. In sum- mary, the action of live organisms accelerates damage processes that may eventually lead to unacceptable performance or cause failure.
This paper presents an overview of biodeterioration of the most widely used infrastructure construction materials, discusses the future challenges in this area, and suggests specific directions for needed research. The objectives of this paper are as follows: 1. Outline the significance of biodeterioration for materials used
to construct large infrastructure systems; 2. Describe biodeterioration processes in wood, metals, and re-
inforced concrete; 3. Describe the uncertainties involved in modeling biodeterio-
ration; and 4. Propose new directions for further research.
Definition of Degradation and Biodeterioration
Deterioration is a loss of structural capacity with time as a result of the action of external agents or material weakening. It has many dimensions and depends, among others, on the type of structure, the constitutive material, the environmental conditions, and the operation characteristics. Along these lines, a widely ac-
cepted definition of biodeterioration was proposed by Hueck
1968 as: “any undesirable change in the properties of a material caused by the vital activities of organisms.” Similarly, Rose 1981 defines biodeterioration as the process by which “biologi- cal agents i.e., live organisms are the cause of the structural lowering in quality or value.” It is important to distinguish be- tween biodeterioration and biodegradation, which can be used mistakenly as equals. According to Allsopp et al. 2006, biodeg- radation is concerned with the use of microorganisms to modify materials with a positive or useful purpose while biodeterioration is referred to the negative impact of live-organisms activity.
Classification of Biodeterioration
According to Gaylarde et al. 2003 biodeterioration can be clas- sified into 1. Physical or mechanical; 2. Fouling or soiling aesthetic; and 3. Chemical: 1 assimilatory and 2 dissimilatory. Physical or mechanical biodeterioration refers to all actions that directly affect the component’s material and mechanical proper- ties. This often is related to the process by which live organisms disrupt the material structure by growth or by movement but do not use the material as a food source e.g., root damage, gnawing by rodents. Fouling or soiling i.e., aesthetic deterioration is caused by the presence of organisms, their dead bodies, excreta, or metabolic products forming a microbial layer on the surface of the structure known as biofilm. This deterioration type is primarily associated with the presence of microorganisms causing an unac- ceptable appearance but the performance of the material is not affected. Finally, chemical biodetrerioration can be divided into assimilatory and dissimilatory. The former occurs when the or- ganisms use the structural component as a source of food i.e., carbon and/or energy source, thus modifying the properties of the material e.g., degradation of fuels, metals. In dissimilatory chemical biodeterioration, on the other hand, the live organisms’ excreted waste products or other substances e.g., H2S, FeS ad- versely affect the material.
Cost of Biodeterioration
The economic consequences resulting from biodeterioration are difficult to quantify and to the best knowledge of the writers, there is little reliable information on this topic. Challenges in estimating the costs associated with biodeterioration are related to the following issues: 1. Biodeterioration is difficult to separate from other damage
processes. In most cases, biodeterioration accelerates other damage mechanisms, which may eventually become the ac- tual cause of unacceptable performance or failure of the structure;
2. The consequences of biodeterioration are not easy to assess at a given time. Biodeterioration is not a continuous process and depends upon changes in climatic as well as on other environmental conditions; and
3. The engineering community is not familiar with biodeterio- ration mechanisms; therefore, in many cases, damage identi- fication focuses only on well known failure mechanisms, overlooking the possible influence of live organisms.
Despite these difficulties, several studies recognize the exis- tence of biodeterioration and the potential impact on the
economy. In the case of wood construction, cost estimations re-
ported by several authors state that the replacement of decayed wood alone consumes 10% of the timber cut annually in the United States; this does not include cost of replacement, liability, and cost of preservative treatment. In 1988, this value was esti- mated to be $613 million Anderson 1990. Currently, it is esti- mated that subterranean termites only, which are the most destructive insect pests of wood in the United States, cause more than $2 billion in damage each year. This is more property dam- age than that caused by fire and windstorm combined. Similar figures have been reported all over the world, for instance, Sand and Bock 1991 found that 1% of the cost of buildings in Ham- burg, Germany must be spent each year on maintenance due to effects of deterioration arising from physical, chemical, and bio- logical attacks approximately $25–$30 billion. In addition to usual maintenance costs, extreme environmental events such as hurricanes and tropical storms may also create the conditions for biodeterioration to take place. Reinsurance companies such as Munich-Re Group 2005 state that following a hurricane, mold damage is inevitable and the long-term consequences have proven to be very expensive.
On the other hand, information about the direct cost of biode- terioration on reinforced concrete structures is almost nonexistent. In the case of steel structures, some estimates have been made in certain areas e.g., for marine structures but the data are not reliable. A study conducted by CC Technology Laboratories, Inc. 2001 estimated the total direct cost of corrosion in infrastructure in the United States is close to $137.9 billion annually. Experi- ence has shown that a significant percentage of corrosion prob- lems are related to microbially induced corrosion.
Based on the estimation of costs mentioned above, it becomes clear that the direct consequences of biodeterioration, although largely uncertain, are well above what the engineering community might think. These figures certainly have a significant impact on the life-cycle costs of large infrastructure systems that cannot be overlooked.
Dynamics of Live-Organism Attacks
New infrastructure components are highly resistant to the direct attack of microorganisms due to the fact that: 1 the potential microbial nutrients are not readily supplied by the materials; and 2 infrastructure is usually found in environmental conditions that restrict microbial growth e.g., high pH and temperature. However, as part of normal structural deterioration and environ- mental changes, biodeterioration may become a hazard whose consequences may result in significant losses. Since biodeteriora- tion is concerned with live organisms, the dynamic nature of the environmental conditions such as variations in humidity and tem- perature, the availability of nutrients, and the permanent move- ment of species are very important. Any attempt to realistically model biodeterioration attack must include time-dependent con- siderations as well as individual characteristics of the organisms involved.
The most common live organisms associated with biodeterio- ration of construction materials are as follows: 1. Marine borers e.g., gribble and shipworms; 2. Insects e.g., termites and wood-boring beetles; 3. Fungi soft rots, white and brown rots, primary and second-
ary molds, stainers algae, and lichens; and 4. Microorganisms e.g., bacteria
The action of marine borers focus mainly on wood structures
such as wooden piers and harbor piles, ships, barriers, and other
OF MATERIALS IN CIVIL ENGINEERING © ASCE / MAY 2008 / 353
forms of wood in marine environments. Although there are many species of marine borers, the major wood borers are the gribble crustacean. Some marine borers do not use wood itself as a food source, but rather search for microscopic algae, bacteria, and soft- rot fungi located in and on the wood. Others, such as shipworm mollusk, digest cellulose. The consequences of most marine borers on steel structures are minor. In concrete structures, marine borers participate actively in the erosion of the concrete surface and may eventually accelerate crack growth rate. The action of other large marine borers, which is restricted to very specific cases, is beyond the scope of this paper.
Insects have a substantial effect on wood structures but not on concrete or metallic materials. Many insects use wood structures based on seasonal requirements; for instance, bees, wasps, ear- wigs, and many others used it as shelter. The two main types of insects affecting wood structures are termites i.e., Isopera and wood-boring beetles Coleoptera. The effect of termites in re- gions where wood construction is common is on the order of a billion United States dollars annually and in the tropics, mainte- nance costs may reach a value of 10% of the property each year Allsopp et al. 2006.
Biodeterioration is usually concerned with the consequences of relatively small living organisms i.e., microorganisms and fungi. The existence and growth of microorganisms requires ap- propriate environmental conditions such as the availability of water, light, oxygen, and nitrogen; all within an environment with the appropriate temperature and pH. The water requirement for microorganisms is expressed by the so-called water activity of the environment aw. The water activity is defined as: lnaw =− ·m · /55.5; where number of ions formed by each sol- ute molecule; mmolar concentration of solute; and molar osmotic coefficient Rose 1981. Pure water has a value of aw
=1.0 and this value decreases when solutes are dissolved in it. Microorganisms can grow in media with 0.63aw0.99. It is known that bacteria require values of 0.93aw0.99, while yeast or molds grow in lower values of 0.88aw0.91. In addi- tion to water availability, microbial invasion also requires the ex- istence of nutrients. Apart from light, the two major classes of nutrients are those that provide a source of energy and nitrogen. They are provided by the enzymatic breakdown of compounds in the materials and by the environment.
Consequences of Action of Live Organisms on Structural Materials
General Considerations Wood is the most common material used in one- and two-story residential construction in North America and in many developed countries Kim et al. 2006. The low durability of wood construc- tion is mainly caused by the lack of attention given to construc- tion details that favor the growth of microorganisms, which, in the long run, weaken the main structural system and affect severely the exterior walls Carll 2000. For instance, the sheathing and framing members permanently absorb free water from condensa- tion or leaks around the perforations of the building envelope Kim et al. 2006. Then, as air flows through the exterior wall
cavity and is restricted by various combinations of air barriers,
354 / JOURNAL OF MATERIALS IN CIVIL ENGINEERING © ASCE / MAY 20
vapor barriers, sealants, and insulation, walls tend to stay wet for longer periods, providing an opportunity for decay fungi to be- come established Smulski 2000a,b.
Conditions Necessary for Wood Deterioration Wood deterioration due to the action of live organisms results from the relationship between the internal wood characteristics and the surrounding environment. Wood deterioration depends significantly on the presence of water. The amount of water stored in a wood component is measured in terms of the moisture content, which is a relationship between the weight of water con- tained in the wood to the dry weight of the wood element. Labo- ratory testing has shown that optimal wood moisture levels for most decay fungi are between 40 and 80% Scheffer 1973. As long as wood structures are kept dry i.e., moisture content below 20% damage as a result of the action of microorganisms is un- likely Levy and Dickinson 1981. On the other hand, timber that is kept permanently wet e.g., marine structures is also at little risk of decay. The greatest hazard for wood structures is in ground contact or in environments with well defined wet and dry cycles. In addition, the orientation of fibers has been found to have a marked effect on the internal movement of water having an im- pact on the colonization of wood by fungi Corbett 1965. Water flows permanently within the wood structure increasing local moisture and oxygen concentrations that may favor the actions of different microorganisms. Aerobic microorganisms require free atmospheric oxygen to survive, while anaerobic microorganisms can grow without the presence of oxygen; therefore, in anaerobic regions only bacteria are usually present, while in regions with appropriate oxygen and humidity, fungal activity can be significant.
In addition to the presence of oxygen and water, most biologi- cal activity requires the presence of nutrients. The availability of nutrients is closely related to the ratio of carbon to nitrogen in wood. When this ratio is very high, the low availability of nitro- gen reduces the potential of fungi to attack the wood. The nitro- gen content of wood ranges from 0.03 to 1%, whereas in other plants this value ranges between 1 and 5%. Other factors that favor the growth of microorganisms i.e., fungi are pH values between 3 and 6 and temperatures in the range of 0–45°C, al- though the ideal temperatures for fungi growth are between 15 and 45°C.
Wood Damage Mechanisms Wood deterioration results from the destruction of: 1 cellulose; 2 hemicellulose; or 3 lignin; these are the components that provide wood with its strength. This deterioration may start in standing trees as well as during the postharvest and transportation processes. In most cases, once any of the biodeterioration mecha- nisms start, the structural resistance decreases very quickly. The biomechanism by which the wood is damaged depends upon the type of organism. This section describes briefly how different organisms degrade wood.
The first group encompasses the so-called marine borers which are very dangerous for wood ships and wood structures built in ocean environments such as wharves, jetties, and breakwaters. The process by which some large marine borers search for larvae and other microorganisms may also scratch the material surface damaging the structural component. In addition, larvae coloniza- tion settles and bores beneath the surface, reducing the structure cross section even further Levy and Dickinson 1981.
A second group of wood degrading agents includes insects
such as Isoptera or termites and wood-boring members of the
Coleoptera or wood-boring beetles. Termites can be found in tropical and subtropical regions and comprise a large number of species that can be divided into: 1 dry wood termites and 2 subterranean termites Rose 1981. Termites construct nests inside timber removing much of the internal wood. It is important to point out that wood-boring insects should be mentioned in any account of microbial deterioration of wood, since many exhibit a form of symbiosis with bacteria and fungi without which they are unable to complete their life cycle.
Within the third group there are smaller organisms usually grouped in the form of molds, which can be divided into primary and secondary molds. Primary molds consist of fungi and they do not degrade the wood cell wall significantly; however, they are very active colonizers. Secondary molds can be more active on wood structures but only after partial breakdown of the wall by other fungi Levy and Dickinson 1981. Within the same cat- egory, but different from molds are the stainers, which are char- acterized by the pigmentation of the hyphal walls usually black or brown in color. Some of these species appear to be capable of causing soft rot. Soft rot is a type of fungus that penetrates into the wood forming chains of cavities that weaken the structure of the material Fig. 1a.
Finally, the wood-rotting Basidiomycetes are the most com- mon and aggressive microorganisms. They are classified as dry- rot and wet-rot fungus. Dry rots tend to be yellow and white, while wet rot are more green-brown; commonly, they are called white and brown rots, respectively. The former i.e., dry rot can attack the wood at a lower water content about 25%, while in most other types of decay these values are about 50%. White rots completely destroy both cellulose and lignin. The dry-rot fungus is very aggressive and can travel over brickwork and masonry and can penetrate plaster and mortar. This type of fungus requires conditions of…